Phase transition in the extreme: a cubic-to-triclinic symmetry change in dielectrically switchable cyanide perovskites.
Trzebiatowska, Monika; Gągor, Anna; Macalik, Lucyna; Peksa, Paulina; Sieradzki, Adam; Dalton transactions (Cambridge, England : 2003) 48 (2019) 15830–15840; doi:10.1039/c9dt03250a

data_7701144
_publ_section_title
;
 Phase transition in the extreme: a cubic-to-triclinic symmetry change in
 dielectrically switchable cyanide perovskites.
;
_journal_issue                   42
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              15830
_journal_page_last               15840
_journal_paper_doi               10.1039/c9dt03250a
_journal_volume                  48
_journal_year                    2019
_chemical_formula_sum            'C8 H10 Co K N10'
_chemical_formula_weight         344.29
_space_group_crystal_system      cubic
_space_group_IT_number           225
_space_group_name_Hall           '-F 4 2 3'
_space_group_name_H-M_alt        'F m -3 m'
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2019-05-21 deposited with the CCDC.    2019-09-16 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.6057(4)
_cell_length_b                   11.6057(4)
_cell_length_c                   11.6057(4)
_cell_measurement_reflns_used    770
_cell_measurement_temperature    330.03(16)
_cell_measurement_theta_max      24.4860
_cell_measurement_theta_min      3.4880
_cell_volume                     1563.20(9)
_computing_cell_refinement       'CrysAlisPro 1.171.38.43 (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.38.43 (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.38.43 (Rigaku OD, 2015)'
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_diffrn_ambient_environment      air
_diffrn_ambient_temperature      330.03(16)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 10.6249
_diffrn_detector_type            Atlas
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.986
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Atlas'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0321
_diffrn_reflns_av_unetI/netI     0.0154
_diffrn_reflns_Laue_measured_fraction_full 0.990
_diffrn_reflns_Laue_measured_fraction_max 0.986
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            1716
_diffrn_reflns_point_group_measured_fraction_full 0.990
_diffrn_reflns_point_group_measured_fraction_max 0.986
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.020
_diffrn_reflns_theta_min         3.040
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    1.368
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.77945
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.38.43 (Rigaku Oxford Diffraction, 2015)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_density_diffrn    1.420
_exptl_crystal_description       plate
_exptl_crystal_F_000             656
_exptl_crystal_size_max          0.025
_exptl_crystal_size_mid          0.020
_exptl_crystal_size_min          0.001
_refine_diff_density_max         0.290
_refine_diff_density_min         -0.129
_refine_diff_density_rms         0.058
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.786
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     17
_refine_ls_number_reflns         141
_refine_ls_number_restraints     14
_refine_ls_restrained_S_all      0.750
_refine_ls_R_factor_all          0.0376
_refine_ls_R_factor_gt           0.0326
_refine_ls_shift/su_max          0.032
_refine_ls_shift/su_mean         0.006
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0967P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0871
_refine_ls_wR_factor_ref         0.0912
_reflns_Friedel_coverage         0.000
_reflns_number_gt                124
_reflns_number_total             141
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c9dt03250a2.cif
_cod_data_source_block           330_CCDC1
_cod_depositor_comments
'Adding full bibliography for 7701143--7701146.cif.'
_cod_original_cell_volume        1563.21(16)
_cod_database_code               7701144
_shelx_shelxl_version_number     2018/3
_oxdiff_exptl_absorpt_empirical_full_min 0.895
_oxdiff_exptl_absorpt_empirical_full_max 1.143
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_shelx_res_checksum              59595